Applying a punch with microridges in multistage deep drawing processes
© The Author(s) 2016
Received: 17 February 2016
Accepted: 23 September 2016
Published: 6 October 2016
The developers of high aspect ratio components aim to minimize the processing stages in deep drawing processes. This study elucidates the application of microridge punches in multistage deep drawing processes. A microridge punch improves drawing performance, thereby reducing the number of stages required in deep forming processes. As an example, the original eight-stage deep forming process for a copper cylindrical cup with a high aspect ratio was analyzed by finite element simulation. Microridge punch designs were introduced in Stages 4 and 7 to replace the original punches. In addition, Stages 3 and 6 were eliminated. Finally, these changes were verified through experiments. The results showed that the microridge punches reduced the number of deep drawing stages yielding similar thickness difference percentages. Further, the numerical and experimental results demonstrated good consistency in the thickness distribution.
KeywordsAspect ratio Finite element method Microridge Multistage deep drawing
The forming processes of sheet metals are advantageous for increasing the rate of production, decreasing the processing costs, improving the quality, and enhancing the yields of mechanical products and are thus widely applied in automotive manufacturing and various industrial products (i.e., electronic, information, and communication products). Recently, industries have emphasized product miniaturization, in which strength and reliability must be considered. This converts the forming processes of thin sheet metals into potential technologies for micro/meso component production technologies.
During microforming, the grain size of the drawing material affects the forming properties in reduced component dimensions; this is referred to as the size effect (Armstrong 1961). Several published articles have described endeavors to improve the drawability of the micro deep drawing process. Erhardt et al. (1999) proposed the concept of warm microforming processes using an Nd/YAG laser to heat sheet metal workpieces locally, thereby reducing the drawing force and increasing the formability. Yagami et al. (2007) utilized a cylindrical cup drawing experiment to investigate the influence of controlling the blank holder motion on removing wrinkles and improving drawability.
In the drawing process, the sheet metal and punch are in close contact with each other when entering the die cavity. During this process, the sheet metal slides through the blank holder and lower die surface. Therefore, friction must be increased between the sheet metal and punch or decreased between the metal sheet and blank-holder or lower die to improve formability (Gong et al. 2011). Gong et al. (2011) used a diamond-like carbon coated blank holder and lower die in a cylindrical cup microforming experiment to reduce friction between the metal sheet and lower die and the blank holder, thereby enhancing formability. Additionally, the micro-features can be used to change the physical properties of the contact surface of the material (Segu and Kim 2014). Steinhoff et al. (1996) investigated the use of deterministic and stochastic surface structures in strip drawing processes. The experimental result shows that the hydrostatic lubrication pockets results in a considerable improvement of the tribological behaviour. Costa and Hutchings (2009) studied the friction effects of controlled surface patterning in tribological situations by using the strip drawing test. The result shows that the relative orientation between the pattern and the drawing direction strongly influenced the friction performance. Moreover, Lin et al. (2015) adopted a microridge punch design that increased not only the friction between the sheet metal and the punch but also the pulling force of the microridges on the sheet metal, distributing the pulling force of the punch on the sheet metal to the microridges. This dispersed the pulling force at the nasal fillet of the punch on the sheet metal and substantially increased drawability.
Numerous researchers have studied the multistage deep drawing process. To confirm the reliability of the finite element analysis of the multistage rectangular cup drawing process, Ku et al. (2002) compared the results obtained from a simulation with the results of an experiment. In multistage elliptical cup deep drawing processes, Kim et al. (2001) used finite element inverse analysis to modify the original die design by enhancing the discrepancy in the thickness strain distribution for each intermediate die shape. With the aid of the finite element analysis, Kim et al. (2002) modified the rectangular cup with a large aspect ratio design to achieve smooth deformation and reduce the possibility of failure in the multistage drawing and ironing process. To lower the possibility of deformation failure, Kim and Hong (2007) designed and implemented a finite element simulation-based search algorithm to determine the optimal design variables of a multistage circular cup drawing process for a molybdenum sheet. To achieve a limiting drawing ratio of 9 for cylindrical brass cups, Faraji et al. (2010) used a limited number of annealing cycles during multistage deep drawing processes. Furthermore, Gau et al. (2013) conducted one deep drawing and two ironing stage experiments using 0.2 mm-thick 304 stainless steel sheets to investigate the effects of processing size. The experimental results showed that varying material annealing temperatures affected the forming heights.
The manufacture of cups with high aspect ratios involves numerous deep drawing stages, which results in high manufacturing costs. Therefore, the design goal of these processes is to reduce the number of stages. However, most published articles have focused on reducing the possibility of failure in the multistage deep drawing process.
This study applied the microridge punch in multistage deep drawing to reduce the number of processing stages. The original eight-stage deep forming process of a copper cylindrical cup with high aspect ratio was exemplified by introducing microridge punch designs to Stages 4 and 7 of the forming process, replacing the original punches and eliminating Stages 3 and 6. Subsequently, the feasibility of the new process was assessed using DEFORM 2D and confirmed through a physical experiment.
Design and analysis of the cylindrical cup multistage forming process
Die design parameters and their values
Original/modified design values
Punch diameter (mm)
Punch nose radius (mm)
Lower die shoulder radius (mm)
Drawing ratio (%)
During the cylindrical cup drawing process, Stage 2 was completed, Stage 3 was eliminated, and Stage 4 (drawing) was executed.
The right side of Fig. 3 shows several microridge rings on the sidewall surrounding the punch nose. These features increase the pulling force on the blank as well as the friction between the blank and punch by distributing the drawing force on the blank from the nasal fillet of the punch to the microridges. Consequently, the drawing force on the blank is no longer concentrated at the punch nose but is distributed through the punch nose and microridges. This slows sidewall thinning, preventing the occurrence of cracks.
The original design presents no cracks when Stages 3 and 4 are performed by using two microridge-free punches. However, in this example, Sage 3 is eliminated to follow the modified design. When Stage 4 is performed by using one microridge-free punch, the part will crack in this stage. In opposition, when Stage 4 is performed by using one microridge punch, the part presents no crack.
Lin et al. (2015) showed that a microridge punch increased deep drawing height by at least 100 % compared with a microridge-free punch in a single-stage deep-drawing process. This paper extends those results to explore the multistage deep drawing of two microridge punches. Specifically, a two-stage deep drawing using two microridge-free punches was replaced with a single-stage deep drawing using a microridge punch to reduce the number of deep drawing stages required.
The procedures involved in modifying the die design process are outlined in the following steps. First, CATIA was adopted to construct 3D models of the original eight-stage deep-drawing dies of copper cups according to the sizes of the dies at each deep-drawing stage. The 3D models were converted into axisymmetric 2D diagrams, and the diagrams were subsequently imported into DEFORM to analyze the formability of each stage of the original deep-drawing processes.
Next, the drawing stages that involved the use of a microridge punch were distributed evenly in the multistage forming processes. Moreover, because the microridge of the punch indents the inner wall of the cylindrical cup during deep drawing processes, the final drawing stage is designed using a microridge-free punch to decrease the indent in the final product. Hence, in the modified design, the microridge punch was designed in Stages 4 and 7 to replace the original punch, and Stages 3 and 6 were eliminated.
Finally, the design parameters (namely ridge height, ridge clearance, ridge nose radius, ridge shoulder radius, ridge-to-punch nose distance, and number of ridges) were specified for the microridge punch. An excessively high ridge height induces the ridges to be deeply pressed into the blank, whereas an extremely low ridge height causes the ridges to generate unsatisfactory drawing effects. Moreover, an extremely high ridge clearance results in the excessive distribution of the ridge drawing force to the blank. The minimum ridge clearance is limited to the thickness of the grinding blade. An extremely long ridge nose radius reduces the drawing force of the ridges; however, an excessively short ridge nose radius causes the ridge to be deeply pressed into the blank. In addition, an excessively long ridge shoulder radius induces the ridges to deliver limited drawing force. The minimum ridge shoulder radius is limited to the nasal fillet radius of the grinding blade. An extremely long ridge-to-punch nose distance results in increased thickness difference percentages, whereas an excessively short ridge-to-punch nose distance leads to changes in the appearance of components. In addition, an extremely high number of ridges increases the punch manufacturing costs, whereas an extremely low number of ridges reduces the drawing effect.
Dimensions of the punch with microridges
Punch diameter, DP (mm)
Punch nose radius, RP (mm)
Ridge height, HR (mm)
Ridge clearance/ridge number
Ridge nose radius, RRN (mm)
Ridge shoulder radius, RRS (mm)
Ridge to punch nose distance, LF (mm)
Finite element analysis of copper cup drawing
This study investigated the copper cylindrical cup multistage deep drawing process by using a microridge punch to reduce the number of stages. During the deep drawing process, the microridges are pressed into the blanks to generate the drawing force. Therefore, this study adopted the commercial software DEFORM to analyze the multistage micro deep drawing process of copper cylindrical cups.
Chemical composition of copper alloy C26800 (wt%)
The FEM model mainly included the components of drawing punches with and without microridge features, a lower die, a blank holder, and a blank. The die components and products exhibited axial symmetry; therefore, 2D axisymmetric elements were adopted in the simulations. The geometric parameters of the multistage deep drawing dies comprised the punch diameter, punch nose radius, lower die shoulder radius, and die clearance. The relevant parameters and values are shown in Table 1. In addition, the modified microridge punch dimensions for Stages 4 and 7 are shown in Fig. 4 and Table 2.
Multistage micro deep drawing experiment
A section of 0.2 mm-thick rolled C26800 copper alloy sheet metal was used as the test material. Cylindrical blanking dies were employed to cut 10.5 mm-diameter cylindrical blanks from the test material. To obtain quality blanks and prevent deckle edges, the clearance between the lower die and cutting punch was 1.5 % of the material’s thickness.
To verify if the microridge punch could reduce the number of forming stages, this experiment first adopted the eight-stage process, using microridge-free drawing punches. Next, a six-stage process was adopted by introducing a microridge punch to Stages 4 and 7 and eliminating Stages 3 and 6.
The multistage micro deep forming test was conducted at room temperature through the following steps: (a) The cylindrical blanks were wiped clean. (b) The blanks were positioned on the V-shaped conical openings. (c) The deep forming process was conducted using punches with and without microridge designs at a forming velocity of 10 mm/min. (d) The semifinished blank products were transferred to the next lower die cavity and positioned on the cylindrical guide. (e) Steps (c) and (d) were repeated until product completion. To reduce friction coefficients, relevant components in each experimental forming stage were adequately lubricated. Additionally, all experiments were repeated at least twice to ensure reproducibility.
Results and discussion
Simulation results of the copper cup
Forming height (mm)
Thickness difference percentage (%)
Maximum deformed load (N)
Thickness of the deformed parts
Because product thickness was low, a wire electric discharge machine was used for sectional processing in each product-forming stage to prevent deformation. The wire electric discharge machine hardened the product surface, affecting measurement quality. Therefore, the hardened surface layer was removed using sandpaper before obtaining relevant measurements. To ensure measurement precision, a confocal microscope was used to measure the cross-sectional thickness of the products for each forming stage.
Microridge punches were designed to decrease the number of stages in the multistage deep drawing process of the high aspect ratio cylindrical cups with the aid of the finite element method. Explicit rigid-plastic finite element analysis with 2D axisymmetric solid elements was performed to calculate the thickness difference percentage in the initial design during the deep drawing process. Guideline of the process design modification was proposed to reduce the number of deep drawing stages at similar thickness difference percentages. The modified design proposed that a two-stage deep drawing using two microridge-free punches was replaced with a single-stage deep drawing using a microridge punch. The deep-drawing process used microridge punches evenly distributed throughout the drawing stages to decrease the indent in the final product. The design parameters of the microridge punches were set based on the comparison of the simulated results with those of the original designs. The modified design was examined by the simulated and experimental results.
A micro multistage deep drawing experiment was conducted in this study to deform 0.2 mm-thick and 10.5 mm-radius C26800 copper alloy sheet metal plates into 2.0 mm-diameter, 15 mm-deep, and 0.16 mm-thick copper cups. Experiments were conducted to compare the forming processes by using a punch nose with and without surface microridge designs. The simulated and experimental results are summarized as follows:
The traditional punch requires eight stages of deep drawing. The modified process involves replacing the microridge-free punches in the original Stages 3–4 and 6–7 by introducing microridge designs in Stages 4 and 7. Specifically, a single processing stage using microridge punch designs replaces two processing stages without using microridge punch designs. Consequently, the microridge designs shorten the eight-stage deep drawing process to a six-stage process.
The experimental testing was conducted according to the simulation results. The comparison showed the thickness distributions demonstrated consistency. Therefore, the commercial forming analysis software accurately simulated the multistage micro deep forming process of the microridge punch designs.
According to the simulated and experimental results, the Stage 8 cups with original and modified designs yielded similar final thickness distributions with maximum thickness difference percentages of approximately 30 %.
BTL conceived the idea and supervised the entire research process. CYY conducted the analysis and experiments. Both authors read and approved the final manuscript.
The authors are grateful for the financial support provided by the Technology Development Program of the Department of Industrial Technology, Ministry of Economic Affairs, Taiwan, ROC (No. 102-EC-17-A-05-S1-218) and the invaluable assistance and advice provided by the Metal Industries Research and Development Centre; GOBO Enterprise Co., Ltd.; Yanzhi Co., Ltd.; and Long Standard Precision Industries Co., Ltd., Taiwan, ROC.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Armstrong RW (1961) On size effects in polycrystal plasticity. J Mech Phys Solids 9:196–199ADSView ArticleGoogle Scholar
- Costa HL, Hutchings IM (2009) Effects of die surface patterning on lubrication in strip drawing. J Mater Process Technol 209:1175–1180View ArticleGoogle Scholar
- Erhardt R, Schepp F, Schmoeckel D (1999) Micro forming with local part heating by laser irradiation in transparent tools. In: Proceedings of the 7th international conference on sheet metal, pp 497–504Google Scholar
- Faraji G, Mashhadi MM, Hashemi R (2010) Using the finite element method for achieving an extra high limiting drawing ratio (LDR) of 9 for cylindrical components. CIRP J Manuf Sci Technol 3:262–267View ArticleGoogle Scholar
- Gau JT, Teegala S, Huang KM, Hsiao TJ, Lin BT (2013) Using micro deep drawing with ironing stages to form stainless steel 304 micro cups. J Manuf Process 15:298–305View ArticleGoogle Scholar
- Gong F, Guo B, Wang C, Shan D (2011) Micro deep drawing of micro cups by using DLC film coated blank holders and dies. Diam Relat Mater 20:196–200ADSView ArticleGoogle Scholar
- Kim HK, Hong SK (2007) FEM-based optimum design of multi-stage deep drawing process of molybdenum sheet. J Mater Process Technol 184:354–362View ArticleGoogle Scholar
- Kim SH, Kim SH, Huh H (2001) Finite element inverse analysis for the design of intermediate dies in multi-stage deep-drawing processes with large aspect ratio. J Mater Process Technol 113:779–795View ArticleGoogle Scholar
- Kim SH, Kim SH, Huh H (2002) Tool design in a multi-stage drawing and ironing process of a rectangular cup with a large aspect ratio using finite element analysis. Int J Mach Tool Manuf 42:863–875View ArticleGoogle Scholar
- Ku TW, Ha BK, Song WJ, Kang BS, Hwang SM (2002) Finite element analysis of multi-stage deep drawing process for high-precision rectangular case with extreme aspect ratio. J Mater Process Technol 130–131:128–134ADSView ArticleGoogle Scholar
- Lin BT, Huang KM, Kuo CC, Wang WT (2015) Improvement of microdeep drawability by using punch surfaces with microridges. J Mater Process Technol 225:275–285View ArticleGoogle Scholar
- Segu DZ, Kim SS (2014) Influence on friction behavior of micro-texturing under lubricated non-conformal contact. Meccanica 49:483–492View ArticleMATHGoogle Scholar
- Steinhoff K, Rasp W, Pawelski O (1996) Development of deterministic-stochastic surface structures to improve the tribological conditions of sheet forming processes. J Mater Process Technol 60:355–361View ArticleGoogle Scholar
- Yagami T, Manabe K, Yamauchi Y (2007) Effect of alternating blank holder motion of drawing and wrinkle elimination on deep-drawability. J Mater Process Technol 187–188:187–191View ArticleGoogle Scholar